Einfache Methoden um Silber auf Echtheit zu prüfen

Wie bestimme ich mit einfachen Mitteln die Echtheit von Silbergegenständen

Wie bestimme ich mit einfachen Mitteln die Echtheit von Silbergegenständen

Einfache Methoden um Silber auf Echtheit zu prüfen

Einleitung

Um Silberbarren, Schmuck oder Münzen auf den Silbergehalt zu prüfen sind normaler Weise sehr aufwendige Verfahren notwendig.

Verfahren wie die Röntgenfluoreszenzspektroskopie und Strichproben mit chemischen Nachweisverfahren weisen immer nur das Metall, welches sich an der Oberfläche befindet nach. Was im Kern liegt bleibt meist verborgen.

Als Garant der Echtheit wird in der Regel die Punzierung der Silbergegenstände angesehen. Aber auch hier ist es mit einfachen Mitteln möglich Fälschungen zu erstellen.

Die vorliegende Anleitung zeigt auf, wie mit einfachen Mitteln, welche in fast jedem Haushalt zur Verfügung stehen oder für wenige Euro angeschafft werden können ohne großen Aufwand eine sichere Aussage über den Silbergehalt von Gegenständen erstellt werden kann.

Um ein grundlegendes Verständnis von versilberten oder silbernen Gegenständen zu schaffen werden die üblichen Legierungen und Kennzeichnungen von Silbergegenständen erläutert und erklärt.

Historisches

Um die Echtheit von Silbergegenständen zu überprüfen, wurden im Mittelalter Farbe, Klang und Gewicht in Augenschein genommen. Zum Nachweis von Silber in Legierungen diente den Goldschmieden die sog. Strichprobe. Dabei wurde das Metall über einen Schwarzschieferstein gerieben und auf den entstandenen weißen Strich ein Tropfen „Silberprobierwasser- (Salpetersäure, HNO₃-saure Kaliumdichromat-Lösung) gegeben. Rotfärbung zeigte Silber an.

Silberlegierungen

Reines Silber ist für Gebrauchsgegenstände viel zu weich. Schon im Altertum wurde Silber daher mit anderen Metallen legiert. Sehr gut lässt sich Silber mit Gold, Kupfer oder Palladium (ein Palladiumgehalt von 20 bis 30% macht Silber anlaufbeständig) legieren. Das Legieren erhöht zumeist die Härte des Silbers. Nicht legierbar ist Silber mit Eisen.

Wichtige Silberlegierungen

Die wichtigsten Silberlegierungen sind heute Kupfer-Silber-Legierungen. Sie werden in der Regel nach ihrem Feingehalt an Silber in tausendstel, angegeben.

Die gebräuchlichsten Silberlegierungen haben einen Feingehalt von 800 und 925 tausendstel Teile Silber.

925er Silber wird nach der britischen Währung Pfund Sterling als Sterlingssilber bezeichnet. Es ist die wichtigste Silberlegierung und wird u. a. zur Herstellung von Münzen, Schmuck und Besteck verwendet.

Eine neuartige Legierung aus England ist Argentium, Sterling Silber, das nicht anlaufen soll. Auch bei stark beanspruchten Bestecken geht seit Jahren der Trend zum Sterlingssilber. Silberwaren werden in der Regel abschließend fein versilbert. Bestecke und Verschleißartikel hart versilbert. Durch die reine Silberbeschichtung werden die verkauf fördernde, strahlendweiße Silberfarbe und ein stark vermindertes Anlaufen der Waren erreicht.

Alpaka ist sehr dünne Versilberung des Trägermaterials Neusilber (der Begriff wird nachfolgend erklärt) mit ca. 15µm Silber. Alpaka lässt sich nicht maschinell spülen. Es läuft schon während des ersten Spülprogramms goldfarben an. Grund hierfür ist der Kupfergehalt der Neusilberlegierung. Die dünne Silberschicht bei Alpaka reicht nicht